LMucko/crystallography-open-database huggingface dataset:
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517914
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O12 S Zn4
;
_chemical_formula_sum            'B6 O12 S Zn4'
_chemical_formula_weight         550.48
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.63458(12)
_cell_length_b                   7.63458(12)
_cell_length_c                   7.63458(12)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    60
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     444.995(12)
_diffrn_ambient_temperature      60
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    15.292
_exptl_crystal_density_diffrn    4.1095(2)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        5.76
_pd_proc_ls_prof_wR_expected     1.30
_pd_proc_ls_prof_wR_factor       9.85
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   7.58
_refine_ls_R_I_factor            1.28
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBOS_60K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        444.99(2)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O12 S Zn4
;
_cod_database_code               4517914
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517915
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O12 S Zn4
;
_chemical_formula_sum            'B6 O12 S Zn4'
_chemical_formula_weight         550.48
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.63706(11)
_cell_length_b                   7.63706(11)
_cell_length_c                   7.63706(11)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    260
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     445.429(11)
_diffrn_ambient_temperature      260
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    15.292
_exptl_crystal_density_diffrn    4.1055(2)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        5.88
_pd_proc_ls_prof_wR_expected     1.30
_pd_proc_ls_prof_wR_factor       9.99
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   7.69
_refine_ls_R_I_factor            1.20
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBOS_260K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        445.43(2)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O12 S Zn4
;
_cod_database_code               4517915
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517916
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O12 S Zn4
;
_chemical_formula_sum            'B6 O12 S Zn4'
_chemical_formula_weight         550.48
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.63467(12)
_cell_length_b                   7.63467(12)
_cell_length_c                   7.63467(12)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    100
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     445.011(12)
_diffrn_ambient_temperature      100
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    15.292
_exptl_crystal_density_diffrn    4.1094(2)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        5.85
_pd_proc_ls_prof_wR_expected     1.30
_pd_proc_ls_prof_wR_factor       9.89
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   7.62
_refine_ls_R_I_factor            1.25
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBOS_100K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        445.01(2)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O12 S Zn4
;
_cod_database_code               4517916
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517917
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O12 S Zn4
;
_chemical_formula_sum            'B6 O12 S Zn4'
_chemical_formula_weight         550.48
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.63563(13)
_cell_length_b                   7.63563(13)
_cell_length_c                   7.63563(13)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    200
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     445.179(13)
_diffrn_ambient_temperature      200
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    15.292
_exptl_crystal_density_diffrn    4.1078(2)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        5.90
_pd_proc_ls_prof_wR_expected     1.30
_pd_proc_ls_prof_wR_factor       10.03
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   7.73
_refine_ls_R_I_factor            1.28
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBOS_200K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        445.18(2)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O12 S Zn4
;
_cod_database_code               4517917
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517918
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O12 S Zn4
;
_chemical_formula_sum            'B6 O12 S Zn4'
_chemical_formula_weight         550.48
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.63757(12)
_cell_length_b                   7.63757(12)
_cell_length_c                   7.63757(12)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    280
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     445.518(12)
_diffrn_ambient_temperature      280
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    15.292
_exptl_crystal_density_diffrn    4.1046(2)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        6.00
_pd_proc_ls_prof_wR_expected     1.30
_pd_proc_ls_prof_wR_factor       9.98
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   7.70
_refine_ls_R_I_factor            1.23
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBOS_280K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        445.52(2)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O12 S Zn4
;
_cod_database_code               4517918
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517919
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O12 S Zn4
;
_chemical_formula_sum            'B6 O12 S Zn4'
_chemical_formula_weight         550.48
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.63863(12)
_cell_length_b                   7.63863(12)
_cell_length_c                   7.63863(12)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    300
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     445.704(12)
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    15.292
_exptl_crystal_density_diffrn    4.1030(2)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        6.06
_pd_proc_ls_prof_wR_expected     1.29
_pd_proc_ls_prof_wR_factor       9.99
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   7.71
_refine_ls_R_I_factor            1.18
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBOS_300K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        445.70(2)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O12 S Zn4
;
_cod_database_code               4517919
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517920
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O12 S Zn4
;
_chemical_formula_sum            'B6 O12 S Zn4'
_chemical_formula_weight         550.48
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.63456(12)
_cell_length_b                   7.63456(12)
_cell_length_c                   7.63456(12)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    80
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     444.992(12)
_diffrn_ambient_temperature      80
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    15.292
_exptl_crystal_density_diffrn    4.1096(2)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        5.76
_pd_proc_ls_prof_wR_expected     1.30
_pd_proc_ls_prof_wR_factor       9.86
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   7.60
_refine_ls_R_I_factor            1.25
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBOS_80K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        444.99(2)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O12 S Zn4
;
_cod_database_code               4517920